week ending 31 JANUARY 2014

PHYSICAL REVIEW LETTERS

Confined Dissipative Droplet Solitons in Spin-Valve Nanowires with Perpendicular Magnetic Anisotropy Ezio Iacocca,1,* Randy K. Dumas,1 Lake Bookman,2 Majid Mohseni,3,4 Sunjae Chung,1,3 Mark A. Hoefer,2 and Johan Åkerman1,3 1

Physics Department, University of Gothenburg, 412 96, Gothenburg, Sweden Department of Mathematics, North Carolina State University, Raleigh, North Carolina 27695, USA 3 Material Physics, School of ICT, Royal Institute of Technology, Electrum 229, 164 40, Kista, Sweden 4 Department of Physics, Shahid Beheshti University, Evin, Tehran 19839, Iran (Received 19 June 2013; published 29 January 2014) 2

Magnetic dissipative droplets are localized, strongly nonlinear dynamical modes excited in nanocontact spin valves with perpendicular magnetic anisotropy. These modes find potential application in nanoscale structures for magnetic storage and computation, but dissipative droplet studies have so far been limited to extended thin films. Here, numerical and asymptotic analyses are used to demonstrate the existence and properties of novel solitons in confined structures. As a nanowire’s width is decreased with a nanocontact of fixed size at its center, the observed modes undergo transitions from a fully localized two-dimensional droplet into a two-dimensional droplet edge mode and then a pulsating one-dimensional droplet. These solitons are interpreted as dissipative versions of classical, conservative solitons, allowing for an analytical description of the modes and the mechanisms of bifurcation. The presented results open up new possibilities for the study of low-dimensional solitons and droplet applications in nanostructures. DOI: 10.1103/PhysRevLett.112.047201

PACS numbers: 75.78.Cd, 85.75.-d

Spin transfer torque (STT) induced excitations in magnetic systems [1–3] have attracted significant attention during the past decade due to their interesting fundamental properties and potential for technological impact. STT can, e.g., be exerted by a spin-polarized current impinging upon a magnetic thin film or by current flow within a magnetically inhomogeneous sample [4]. The former is achieved in devices known as spin valves (SVs) [5–8], where two magnetic layers are separated by a nonmagnetic spacer. One of the magnetic layers is considered largely insensitive to external excitations (fixed), and spin polarizes the applied dc current. The second (free) magnetic layer is subjected to STT, giving rise to currenttunable dynamical modes such as propagating spin waves [9–13], localized spin-wave bullets [12–17], vortices [18–20], and dissipative droplets. [21–23] The required high current densities are usually achieved by patterning a nanocontact (NC) on top of the spinvalve (NC-SV). On the other hand, STT induced by currents within a magnetically inhomogeneous sample provides the basis for current-induced domain-wall motion [24,25], as demonstrated in nanowire ferromagnetic thin films [26–28] and SVs [29,30]. For both types of STT excitations, perpendicular magnetic anisotropy (PMA) materials are of fundamental and technological interest. PMA materials support topological (Skyrmions) [31,32] and nontopological (magnetic dissipative droplets) [21,23] solitons, which offer a novel approach to applications [33–36] and control methods [22,37–39]. In particular, the magnetic dissipative droplet (“droplet” in the following) features a dynamical nature recently studied theoretically [21,22,37] and experimentally [23]. However, 0031-9007=14=112(4)=047201(5)

these studies have considered only two-dimensional (2D) thin films, so it is natural to inquire about the role of physical confinement that nanoscale applications would introduce. For this, we investigate the effect of lateral confinement on droplets with micromagnetic simulations and asymptotic methods. This Letter describes how a droplet undergoes transitions to an edge droplet and then to a quasi-one-dimensional (quasi-1D) droplet as an extended magnetic thin film is reduced to a nanowire. The edge droplet is essentially a nontopological half 2D droplet, exhibiting a larger footprint with respect to the NC. On the other hand, the quasi-1D droplet establishes oscillating magnetic boundaries along the physically extended dimension of the nanowire and it is found to acquire a chirality consistent with soliton-soliton pairs that exhibit breathing, similar to 1D solitons in biaxial ferromagnets [40,41]. Owing to the above-mentioned features, the mode transitions are evidenced by distinct precessional frequencies. The presented results suggest these novel droplets as candidates for low-dimensional applications and soliton research in an experimentally realizable system. Droplets are two-dimensional, nontopological modes sustained by the STT-induced creation of an effective zero damping region below the NC, i.e., a gain-loss balance. In such a region, the magnetization is mostly reversed, creating a dynamic magnetic boundary with its environment (Fig. 1). This boundary defines the droplet size and it is expected to be strongly affected by lateral confinement. In order to explore such consequences, we begin by performing micromagnetic simulations of nanowires of

047201-1

© 2014 American Physical Society

PRL 112, 047201 (2014)

PHYSICAL REVIEW LETTERS

FIG. 1 (color online). 2D droplet excited in an extended spin valve, showing its mostly reversed core. Below, the schematic of the spin valve is shown, where the nonmagnetic spacer is identified in ochre while the PMA material coloring follows the mz component as indicated in the color bar. The nanocontact is placed in the geometrical center of the simulated area.

decreasing width while keeping the NC laterally centered and of fixed radius. The droplet nucleation is due to a spin-wave modulational instability [21] leading to strongly nonlinear dynamics, often requiring micromagnetic simulations to uncover their features. However, an analytical treatment is available when some simplifications are made, as will be discussed below. The system under study is a trilayered NC-SV consisting of PMA free and fixed layers (Fig. 1). Micromagnetic simulations are performed for the free layer with the graphics-processing-unit-based tool Mumax2 [42], using a second-order Runge-Kutta solver with an adaptive step bounded between 1 fs and 1 ps [13]. The dynamics follow the Landau-Lifshitz-Gilbert-Slonczewski equation ˆ ˆ dm dm ⃗ eff þ αm ˆ × ˆ × μ0 H ¼ −γ m dt dt ˆ ˆ ×m ˆ × M; − γμ0 Ms σðIÞfð ⃗xÞϵm

(1)

ˆ ˆ and M where γ=2π ¼ 28 GHz=T is the gyromagnetic ratio, m are the normalized free and fixed layer magnetization vectors, respectively, α is the Gilbert damping, and σðIÞ ¼ ℏIPλ=μ0 M2s eVðλ þ 1Þ is the dimensionless spin torque coefficient where ℏ is the reduced Planck constant, I is the spinˆ ˆ · MÞ, polarized current, P is the polarization, ϵ ¼ 1=ð1 þ νm ν ¼ ðλ − 1Þ=ðλ þ 1Þ, λ is the spin torque asymmetry, μ0 is the vacuum permeability, Ms is the saturation magnetization, e is the electron charge, and V is the free layer volume. STT is active only within the NC, a disk centered at the origin with diameter d defined by fð ⃗xÞ ¼ 1, j ⃗xj < d=2 and ⃗ eff includes the zero elsewhere. The effective field H exchange, demagnetizing, anisotropy, and an out-of-plane external field μ0 Ha ¼ 0.4 T. The current-induced Oersted field is also included in the simulations by approximating the current flow path as an infinite cylinder. We assume material parameters measured on similar Co/Ni multilayers [23,43]: thickness ¼ 5 nm, α ¼ 0.05, magnetic anisotropy K u ¼ 447 kJ=m3 , Ms ¼ 716.2 kA=m, and exchange stiffness A ¼ 30 pJ=m—similar to Co. The current-polarizing fixed layer is assumed to be perfectly out of plane with spin

week ending 31 JANUARY 2014

torque asymmetry λ ¼ 1.1 and polarization P ¼ 1 for simplicity. The unitary polarization generally leads to an underestimation of the current-induced Oersted field. However, its effect on the presented results is negligible (see the Supplemental Material [44]) and it is only included for completeness. All simulations are performed in the absence of thermal fluctuating fields unless specified. In order to study the effect of lateral confinement, the simulated layer’s length (x axis) is fixed to 1000 nm while the width (y axis) is varied between 300 and 50 nm. The cell size is determined for each nanowire width to boost performance, yet defining an upper limit of 5 nm, below the exchange length λex ≈ 8.2 nm. The NC has a diameter d ¼ 50 nm (Fig. 1) from which current is assumed positive when flowing from the free to the fixed layer. Note that the different cell sizes introduce a discretization error in the STT region, fð ⃗xÞ. However, the robustness of the presented dynamics indicates that such error is negligible. Droplets of a varying nature are excited above the threshold currents shown in Fig. 2(a), determined by the condition hmz ðt > 10 nsÞiNC < 0, where h·iNC indicates average under the NC, while sweeping the current in steps of 0.1 mA. This criterion is motivated by the fact that 2D droplets always contain a significant portion of the magnetization pointing to the southern hemisphere [21]. Figure 2(a) exhibits current local maxima, indicated by arrows, related to standing spin waves across the nanowire width, which preclude the onset of the modulation instability that gives rise to droplets [21]. Consequently, higher currents are needed to induce the spin-wave amplitude growth (see the Supplemental Material [44]). The droplet frequencies are determined from 200 ns time traces sampled at ∼10 ps [Fig. 2(b)], from which three different modes are identified. The frequencies for M1 and M2 lie between the ferromagnetic resonance,

FIG. 2 (color online). (a) Threshold current for droplet nucleation and (b) droplet frequency at threshold as a function of the nanowire width. Three modes are identified: dissipative (M1), edge (M2), and quasi-1D (M3) droplet. The FMR and Zeeman frequencies are shown in black dashed lines. The analytically calculated frequencies are shown in solid red lines.

047201-2

PRL 112, 047201 (2014)

PHYSICAL REVIEW LETTERS

FMR ¼ γμ0 ðHa þ Hk − N z Ms Þ, and Zeeman ¼ γμ0 Ha frequencies—both shown as black dashed lines—where N z is the out-of-plane demagnetizing factor and μ0 Hk ¼ 2K u =Ms ¼ 1.25 T is the anisotropy field [23,43]. These frequency bounds coincide with those for 2D droplets in extended thin films [21]. Contrarily, M3 exhibits a subZeeman frequency. In the following, we investigate the characteristics of each mode by choosing three representative nanowire widths, namely 300 nm (M1), 140 nm (M2), and 50 nm (M3). Their simulated spectra are shown in Fig. 3(a), exhibiting a clean resonance as expected for droplets under a perpendicular external field. These modes exist even when temperature, parameterized as a random thermal field [45] equivalent to 300 K, is included in the simulations. Such spectra are indicated by the subscript T in Fig. 3(a). The observed frequency shift is consistent with the thermally induced tilt of mz towards the plane so that its frequency approaches the Zeeman frequency, in agreement with the dissipative droplet theory [21]. In the absence of thermal fluctuations, a resonant type of M3 is obtained at a nanowire width of 120 nm and identified as a numerical artifact (see the Supplemental Material [44]).

week ending 31 JANUARY 2014

A distinction between the modes can be made from their spatial profiles, shown as contour plots of the mz component [Fig. 3(b)] and surface plots of the mx component [Fig. 3(c)]. These plots confirm that M1 is the 2D droplet discussed in Ref. [21], including the Oersted-induced asymmetric location with respect to the NC. However, below a critical width, M2 arises as an edge mode where the droplet’s footprint increases and “sticks” to the nanowire’s side. The particular location of M2 appears to be random and determined by slight asymmetries, numerical round-off errors, and thermal fluctuations, if included. The edge M2 can be understood as a half 2D droplet (see the Supplemental Material [44]), in analogy to previously studied conservative three-dimensional surface droplets [46]. Furthermore, the Skyrmion number [32,47] of M1 and M2 is N ¼ 0 as predicted by theory, motivating a similar analytical treatment for M2, as we describe below. For the following theoretical discussion, we neglect the symmetry breaking Oersted and long-range demagnetizing fields in order to derive an analytical description. The ˆ boundary conditions accompanying Eq. (1) are ∂ m=∂n ¼ 0 where n is an outward pointing normal. Since the 2D ˆ droplet ¼ m ˆ droplet ðρÞ, droplet is azimuthally symmetric, i.e., m ﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ˆ droplet = ρ ¼ x2 þ y2 , we immediately observe that ∂ m ∂yjy¼0 ¼ 0 along the droplet centerline. This implies that a droplet situated with its centerline at the boundary of the half plane y > 0 is a solution of Eq. (1) and can describe M2 for sufficiently wide nanowires due to exponential localization in x and for y > 0. Consequently, an asymptotic analysis [21] can be used to derive the sustaining current σðIÞ for which zero total energy loss (gain-loss balance) is enforced, as required by all dissipative solitons σðIÞ ¼ −ðH k =Ms − 1Þ½ω0 þ H a =ðHk − Ms Þ α R 2 0 0 y0 >0 sin Θð ⃗x Þd ⃗x ×R ; 2 sin Θð ⃗x0 Þ 0 x02 þðy0 −ðw0 =2ÞÞ2